'NaGdS2: a promising sulfide for cryogenic magnetic cooling'
Delacotte, C.; Pomelova, T.A.; Stephant, T.; Guizouarn, T.; Cordier, S.; Naumov, N.G.; Lemoine, P.; Chemistry of Materials 34 (2022) 1829–1837; doi:10.1021/acs.chemmater.1c04105

data_4004088
_publ_section_title
;
 'NaGdS2: a promising sulfide for cryogenic magnetic cooling'
;
_journal_issue                   4
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1829
_journal_page_last               1837
_journal_paper_doi               10.1021/acs.chemmater.1c04105
_journal_volume                  34
_journal_year                    2022
_chemical_formula_moiety         'Gd Li S2'
_chemical_formula_structural     LiGdS2
_chemical_formula_sum            'Gd Li S2'
_chemical_formula_weight         228.323
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_formula_units_Z            2
_cell_length_a                   5.52988(5)
_cell_length_b                   5.52988(5)
_cell_length_c                   5.52988(5)
_cell_measurement_temperature    293(2)
_cell_volume                     169.101(3)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      293(3)
_diffrn_detector                 'see experimental section'
_diffrn_detector_area_resol_mean 'see experimental section'
_diffrn_detector_type            'see experimental section'
_diffrn_measurement_device_type  'see experimental section'
_diffrn_measurement_method       'see experimental section'
_diffrn_radiation_monochromator  'see experimental section'
_diffrn_radiation_type           X-ray
_diffrn_source                   'Laboratory diffractometer'
_diffrn_source_target            Cu
_pd_meas_2theta_range_inc        0.019654
_pd_meas_2theta_range_max        79.94070
_pd_meas_2theta_range_min        5.00000
_pd_meas_number_of_points        3814
_pd_proc_2theta_range_inc        0.019654
_pd_proc_2theta_range_max        79.8962
_pd_proc_2theta_range_min        4.9555
_pd_proc_ls_prof_R_factor        3.8388
_pd_proc_ls_prof_wR_expected     3.7848
_pd_proc_ls_prof_wR_factor       4.7284
_pd_proc_wavelength              1.540560
_refine_ls_number_parameters     7
_refine_ls_number_reflns         8
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            6.0942
_cod_data_source_file            LiGdS2.cif
_cod_data_source_block           LiGdS2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Cubic' was changed to
'cubic' in accordance with the built-in table derived from the CIF
Core dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21.

Automatic conversion script
Id: cif_fix_values 8738 2021-04-28 16:35:53Z antanas 
;
_cod_original_cell_volume        169.102(3)
_cod_database_code               4004088
_pd_proc_ls_prof_cr_factor       48.4304
_pd_proc_ls_prof_cwr_factor      21.9546
_pd_proc_ls_prof_cwr_expected    17.5735
_pd_proc_ls_prof_chi2            1.5607
_pd_proc_ls_prof_echi2           1.8335